Identification and investigation of new lowdimensional ... · Identiﬁcation and investigation of...
Embed Size (px)
Transcript of Identification and investigation of new lowdimensional ... · Identiﬁcation and investigation of...

Loughborough UniversityInstitutional Repository
Identification andinvestigation of new
lowdimensional quantumspin systems
This item was submitted to Loughborough University's Institutional Repositoryby the/an author.
Additional Information:
A Doctoral Thesis. Submitted in partial fulfillment of the requirementsfor the award of Doctor of Philosophy of Loughborough University.
Metadata Record: https://dspace.lboro.ac.uk/2134/8963
Publisher: c J. M. Law
Please cite the published version.
https://dspace.lboro.ac.uk/2134/8963

This item was submitted to Loughboroughs Institutional Repository (https://dspace.lboro.ac.uk/) by the author and is made available under the
following Creative Commons Licence conditions.
For the full text of this licence, please go to: http://creativecommons.org/licenses/byncnd/2.5/

Identification and investigation of
new lowdimensional quantum spin
systems
by
Joseph M. Law
Doctoral Thesis
Submitted in partial fulfillment of the requirements for the award of
Doctor of Philosophy of Loughborough University
September 27, 2011
c by J. M. Law 2011

Hwt!
Beowulf  Unknown author
circa 8th11th century
i

Abstract
This thesis focuses on one area of modern condensed matter physics,
namely lowdimensional magnetism, and more specifically onedimen
sional linear chains. The work herein can be split into three parts. The
first part provides a tool for the greater community. I herein propose a
Pade approximation for the temperature dependent magnetic suscepti
bility of a S = 3/2 spin chain, that is more accurate than those already
known. The approximation allows one to fit experimentally measured
magnetic susceptibilities and ascertain values such as the nearneighbour
spin exchange interaction and the gfactor. The second and third parts
of this thesis are both concerned with experimentally and theoretically
characterizing two isostructural linear S = 1/2 chain compounds on op
posite ends of the 3d transition metal series. The compounds, CuCrO4
(3d9) and TiPO4 (3d1), are shown to have completely different ground
states despite both being largely isostructural and S = 1/2 quantum
spin systems. In this work and the resulting publications it is shown that
CuCrO4 is a onedimensional S = 1/2 spin chain with antiferromagnetic
nearest and next nearestneighbour spin exchange interactions. The
ratio of these spin exchange interactions is shown experimentally and
theoretically to be approximately 2, putting CuCrO4 in the vicinity of
the MajumdarGhosh point, for which the magnetic groundstate can
ii

be solved analytically. Small ferromagnetic interchain coupling leads
to longrange ferromagnetic ordering between antiferromagnetic chains
at 8.2(2) K. At this temperature a spontaneous electrical polarization
is observed. This classifies CuCrO4 as a typeII multiferroic. Contrary
to CuCrO4, TiPO4 has a nonmagnetic ground state. At 111 and 74 K
TiPO4 undergoes a two stage phase transition, which is interpreted as
a spinPeierls transition. There is evidence that below 74 K TiPO4 has
a new crystal structure, in which there are alternating dimerised chains
and two different PO4 tetrahedral units. Currently the new structure
has not been identified and no superstructure reflections have been con
firmed in either lowtemperature neutron or xray diffraction.
In summary this thesis presents some experimental and theoretical con
tributions to the field of lowdimensional magnetism.
iii

Publication list
1. J. M. Law, C. Hoch, M.H. Whangbo, and R. K. Kremer, Descrip
tion of anhydrous (black) dioptase as a S=1/2 uniform antiferro
magnetic chain system, Zeitschrift fur anorganische und allgemeine
Chemie 636, 54 (2010).
2. J. S. Kim, S. H. Khim, H. J. Kim, M. J. Eom, J. M. Law, R.
K. Kremer, J. H. Shim, and K. H. Kim, Electronhole asymmetry
revealed in the phase diagrams of Fesite doped SrFe2As2, Phys.
Rev. B 82, 024510 (2010).
3. M. Mourigal, M. Enderle, R. K. Kremer, J. M. Law and B. Fak,
Ferroelectricity from spin supercurrents in LiCuVO4, Phys. Rev. B
83, 100409(R) (2011).
4. J. M. Law, C. Hoch, R. Glaum, I. Heinmaa, R. Stern, J. Kang, C.
Lee, M.H. Whangbo, and R. K. Kremer, SpinPeierls transition in
the S=1/2 compound TiPO4 featuring large intrachain coupling,
Phys. Rev. B 83, 180414(R) (2011).
5. A. BussmannHolder, J. Kohler, R. K. Kremer, and J. M. Law,
Analogies of structural instabilities in EuTiO3 and SrTiO3, Phys.
Rev. B 83, 212102 (2011).
iv

6. J. M. Law, P. Reuvekamp, R. Glaum, C. Lee, J. Kang, M.H.
Whangbo, and R. K. Kremer, Quasionedimensional antiferromag
netism and multiferroicity in CuCrO4, Phys. Rev. B 84, 014426
(2011).
7. M. Johnsson, P. Lemmens, J. M. Law, R. K. Kremer, M.H. Whangbo
and K. Y. Choi, Structural and Magnetic Properties of FeTe3O7X
(X=Cl, Br), in preparation, (2011).
v

Contents
1 Magnetism 1
1.1 Magnetism . . . . . . . . . . . . . . . . . . . . . . . . . . 1
1.1.1 The magnetic moment . . . . . . . . . . . . . . . 2
1.1.2 Crystal electric field . . . . . . . . . . . . . . . . 4
1.1.3 Interactions . . . . . . . . . . . . . . . . . . . . . 6
1.1.4 Spin models . . . . . . . . . . . . . . . . . . . . . 9
1.2 Onedimensional magnetism . . . . . . . . . . . . . . . . 10
1.2.1 Multiferroicity . . . . . . . . . . . . . . . . . . . . 13
1.2.2 Some known lowdimensional S = 1/2 quantum
spin chains . . . . . . . . . . . . . . . . . . . . . . 14
1.2.3 Interchain couplings and longrange ordering . . 21
vi

1.2.4 Electron paramagnetic resonance theory . . . . . 22
1.2.5 Pade approximation for the molar magnetic sus
ceptibility of a S = 32 Heisenberg quantum anti
ferromagnetic spin chain . . . . . . . . . . . . . . 25
1.3 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . 32
2 Experimental methodology and computation 33
2.1 Xray and neutron diffraction . . . . . . . . . . . . . . . 34
2.1.1 Single crystal diffraction . . . . . . . . . . . . . . 34
2.1.2 Powder diffraction . . . . . . . . . . . . . . . . . 34
2.2 Magnetisation . . . . . . . . . . . . . . . . . . . . . . . . 36
2.2.1 SQUID magnetometry . . . . . . . . . . . . . . . 36
2.3 Specific heat . . . . . . . . . . . . . . . . . . . . . . . . . 40
2.3.1 Relaxation calorimetry . . . . . . . . . . . . . . . 40
2.3.2 Adiabatic Nernst calorimeter . . . . . . . . . . . 41
2.4 Electron Paramagnetic Resonance spectroscopy . . . . . 42
2.5 Dielectric capacitance . . . . . . . . . . . . . . . . . . . . 45
2.6 Computation . . . . . . . . . . . . . . . . . . . . . . . . 46
vii

2.6.1 Algorithms and Libraries for Physics Simulations
 ALPS . . . . . . . . . . . . . . . . . . . . . . . 46
2.7 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . 47
3 CuCrO4  A new multiferroic material 48
3.1 Crystal structure . . . . . . . . . . . . . . . . . . . . . . 49
3.2 Sample preparation . . . . . . . . . . . . . . . . . . . . . 50
3.3 Magnetic susceptibility . . . . . . . . . . . . . . . . . . . 52
3.4 Specific heat . . . . . . . . . . . . . . . . . . . . . . . . . 60
3.5 Electron paramagnetic resonance . . . . . . . . . . . . . 66
3.6 ab initio calculations . . . . . . . . . . . . . . . . . . . . 72
3.7 Dielectric capacitance . . . . . . . . . . . . . . . . . . . . 77
3.8 Discussion and conclusion . . . . . . . . . . . . . . . . . 81
3.9 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . 83
4 TiPO4  A new spinPeierls system? 85
4.1 Introduction and crystal structure . . . . . . . . . . . . . 85
4.2 Sample preparation . . . . . . . . . . . . . . . . . . . . . 88
viii

4.3 Magnetic susceptibility . . . . . . . . . . . . . . . . . . . 89
4.4 Specific heat . . . . . . . . . . . . . . . . . . . . . . . . . 95
4.5 Electron paramagnetic resonance . . . . . . . . . . . . . 97
4.6 ab initio calculations . . . . . . . . . . . . . . . . . . . . 104
4.7 Magic angle spinning 31P nuclear magnetic resonance and
Raman spectroscopy measurements . . . . . . . . . . . . 109
4.8 Lowtemperature diffraction . . . . . . . . . . . . . . . . 117
4.9 Discussion and conclusion . . . . . . . . . . . . . . . . . 124
4.10 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . 127
5 Conclusion 128
ix

List of Figures
1.1 Taken from magnetism and magnetic materials by J. M.
D. Coey (a): The five orbitals of the 3d transition metals.
(b): The energy splitting of the 3d orbitals (from left to
right); a free atom, an atom in a triangular based pyra
mid environment, an atom in a nondistorted octahedral
environment and an atom in a cubic environment. (c):
The energy landscape of the 3d orbitals in an elongated
(left) and a compressed (right) octahedral environment. 5
1.2 A pictorial representation of the high and lowspin con
figurations for Fe3+. . . . . . . . . . . . . . . . . . . . . . 6
1.3 A graphical representation of the radial wave functions of
the free, bonded and antibonded states of the H2 molecule.
Taken from Magnetism in Condensed Matter Physics by
S. Blundell. . . . . . . . . . . . . . . . . . . . . . . . . . 7
x

1.4 A simplified onedimensional chain of atoms, with the nn
and nnn spin exchange interactions indicated. . . . . . . 11
1.5 A pictorial representation of a frustration in onedimensional
lattice. . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12
1.6 The magnetic susceptibility of a uniform nn Heisenberg
spin chain with Jnn = 1 and a gfactor = 2, calculated
using the Pade approximation put forth by Johnston et al.. 13
1.7 The nn nnn spin exchange phase diagram for S = 1/2
onedimensional system, adapted from Bursill et al.. The
coloured sections/lines are density functional theory cal
culations for real systems, except the line labeled LiCuVO4
INS which is based on an inelastic neutron scattering results. 16
1.8 Main (o): The relative dielectric constant of LiCuVO4 ver
sus temperature. Inset (o): The electrical polarization of
LiCuVO4, calculated from the pyroelectric current, versus
temperature. Taken from Schrettle et al.. . . . . . . . . . 17
1.9 Main (o): The molar magnetic susceptibility of CuCl2
measured in a magnetic field of 1 T versus temperature.
Inset (o): A loglog plot of the specific heat of CuCl2
versus temperature. All results taken from Banks et al.. . 19
xi

1.10 Main (o): The relative dielectric constant of CuCl2 versus
temperature, for various magnetic fields. Inset (o): The
electrical polarization of CuCl2, calculated from the py
roelectric current, versus temperature. Taken from Seki
et al.. . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20
1.11 The electron paramagnetic resonance normalised linewidth
versus reduced temperature for CuGeO3, KCuF3 and NaV2O5
shown against a linear line. The graph is taken from the
work by Oshikawa and Affleck. . . . . . . . . . . . . . . . 23
1.12 (o): Our quantum Monte Carlo results, see text for more
information. Solid blue line: The Pade approximation by
Grossjohann. Solid green line: The classical approxima
tion put forth by Fischer. Solid black line: The approxi
mation by Hiller et al. . . . . . . . . . . . . . . . . . . . 28
1.13 Left: The scaled computation time versus system size at a
reduced temperature of 0.05. Right: The arbitrary com
putation time versus spin, at a reduced temperature of
0.05. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29
xii

1.14 Main: (o): The temperature dependent modified spin sus
ceptibility for a S = 3/2 spin chain with nn spin exchange
interactions, calculated by quantum Monte Carlo using
the ALPS suite, versus reduced temperature. Solid red
line: A fit to a Pade approximation as discussed in the
text. (a): (o): The difference between the modified spin
susceptibility as calculated by quantum Monte Carlo and
the Pade approximation fitted to the simulation. The
solid red lines denotes the boundaries of the error bars
given for the quantum Monte Carlo calculation. (b) The
modified spin susceptibility for different systems sizes at a
fixed reduced temperature of 0.05. N denotes the number
of spins. . . . . . . . . . . . . . . . . . . . . . . . . . . . 30
2.1 Schematic of the powder diffractometer HRPT at the Paul
Scherrer Institute (Switzerland). . . . . . . . . . . . . . . 36
2.2 Left: A filled gelatine capsule as used for measuring the
magnetization. Right: A disassembled, empty, gelatine
capsule, prior to use for measuring magnetization. . . . . 38
xiii

2.3 Left: A filled and sealed quartz tube ready for magnetiza
tion measurements. Right: A closer view of the seal half
way up the tube. . . . . . . . . . . . . . . . . . . . . . . 38
2.4 Top: An empty glass bell jar. Bottom: A full sealed glass
bell jar, ready for specific heat measurements; left is a
view from the top and right is a view from the side. . . . 42
2.5 Left: The electron paramagnetic resonance sample holder
with a mounted temperature sensor. Right: The electron
paramagnetic resonance neutral lowbackground suprasil c
quartz tube with a sample mounted. . . . . . . . . . . . 43
3.1 The crystal structure of CuCrO4, projected slightly off of
the caxis. The unit cell is doubled along the caxis. Blue
octahedra: CuO6 units. Green tetrahedra: CrO4 units. . 49
xiv

3.2 (o): Measured xray powder diffraction pattern of CuCrO4
( = 0.70930 A ). Solid red line: Calculated pattern
(Rp = 13.1%, reduced 2 = 1.15) using the parameters
given in table 3.1. Solid blue line: The offset difference
between measured and calculated patterns. The positions
of the Bragg reflections used to calculate the pattern are
marked by the green vertical bars in the lower part of the
figure. . . . . . . . . . . . . . . . . . . . . . . . . . . . . 52
3.3 The molar magnetic susceptibility of CuCrO4, in the low
temperature regime, versus temperature for various mag
netic fields. Red symbols: Heating data. Blue symbols:
Cooling data. . . . . . . . . . . . . . . . . . . . . . . . . 54
3.4 (o): The inverse molar magnetic susceptibility versus tem
perature of CuCrO4, measured in a field of 7 T. Red solid
line: Fit to the modified CurieWeiss law as given in equa
tion 3.1. . . . . . . . . . . . . . . . . . . . . . . . . . . . 56
3.5 (o): The 7 T molar magnetic susceptibility versus tem
perature for CuCrO4. Dashed/solid lines: The simulated
molar magnetic susceptibility for various cases, see text
for more details. . . . . . . . . . . . . . . . . . . . . . . . 57
xv

3.6 Full diagonalization results. Solid red and black lines are
the magnetisation and d(M)d(H) versus applied magnetic field,
respectively. . . . . . . . . . . . . . . . . . . . . . . . . . 60
3.7 The specific heat versus temperature for CuCrO4. (o):
0 T data. (): 9 T data, offset by +0.5 J/molK. . . . . 62
3.8 (o): The specific heat divided by temperature versus tem
perature for CuCrO4, in the temperature range of the
anomaly. . . . . . . . . . . . . . . . . . . . . . . . . . . . 63
3.9 The specific heat divided by T 3/2 versus T 3/2. (o): Mea
sured data. Solid red line: linear fit, with a slope of
4.31(1) 103 J/molK4 and an intercept of 0.0109(1)
J/molK5/2. . . . . . . . . . . . . . . . . . . . . . . . . . . 65
3.10 (o): Electron paramagnetic resonance signal for CuCrO4
taken at 297(1) K. Solid red line: Fit to equation 2.1. . . 67
3.11 Fitted parameters of the electron paramagnetic resonance
signal of CuCrO4 versus temperature. (a): Intensity of
the electron paramagnetic resonance signal. (b): gfactor.
(c): The half width at half maximum and the solid red
line is a fit to a linear slope, with a gradient of 2.75(2)
T/K and an intercept of 220(5) K. . . . . . . . . . . . . 70
xvi

3.12 (o): Fitted inverse of the integrated electron paramag
netic resonance intensity of CuCrO4 versus temperature.
Solid red line: Linear fit with an arbitrary gradient and
an intercept of 63.1(1) K. . . . . . . . . . . . . . . . . . 71
3.13 (a): Spin exchange pathways used for the mapping for the
density functional theory results. (b): The five spin con
figurations for which the total energy has been calculated
by GGA+U calculations. Shown are the equations used
from mapping the energies onto the aforementioned spin
exchange pathways. Shown below in parentheses are the
relative energies given in meV, first for U = 4 eV and then
for U = 6 eV. . . . . . . . . . . . . . . . . . . . . . . . . 74
3.14 The predicted magnetic structure of CuCrO4, the chemi
cal unit cell is denoted by the dashed box. (a) The mag
netic structure in the ab plane, white and black circles
represent different magnetic moment directions. (b) The
magnetic structure within the acplane, with the mag
netic moments represented by an arrow. . . . . . . . . . 77
xvii

3.15 Main: The temperature dependence of the relative di
electric constant for CuCrO4 at lowtemperatures under
various magnetic fields, refer to legend. (a): A magnetic
isotherm of the relative dielectric constant at 5.2(1) K.
(b): The relative dielectric constant of CuCrO4 at higher
temperatures in zero magnetic field. . . . . . . . . . . . . 80
4.1 The crystal structure of TiPO4, projected slightly off the
caxis. The unit cell is doubled along the caxis. Yellow
octahedra: TiO6 units. Purple tetrahedra: PO4 units. . . 86
4.2 A single crystal of TiPO4. The orientation and size are
indicated. . . . . . . . . . . . . . . . . . . . . . . . . . . 88
4.3 (o): The molar magnetic susceptibility versus tempera
ture for a powder sample of TiPO4 measured in a field of
1 T. Red solid line: Fit to a S = 1/2 Heisenberg antifer
romagnetic chain with a uniform nearestneighbour spin
exchange interaction model, as given by Johnston et al.. 90
xviii

4.4 (o): Heating data. (o): Cooling data. Left: The molar
magnetic susceptibility versus temperature in the region
of the 74 K anomaly. Right: The molar magnetic sus
ceptibility versus temperature in the region of the 111 K
transition. . . . . . . . . . . . . . . . . . . . . . . . . . . 91
4.5 (o): The lowtemperature molar magnetic susceptibility
versus temperature for TiPO4. The red and blue solid
lines are fits of the data using equation 4.1 and the values
tabulated in table 4.1. . . . . . . . . . . . . . . . . . . . 95
4.6 Main (o): The specific heat versus temperature for TiPO4.
Insert (o): The specific heat divided by temperature ver
sus temperature. . . . . . . . . . . . . . . . . . . . . . . 96
4.7 The specific heat of TiPO4 (o): Cooling data. (o): Heat
ing data. Left: The specific heat versus temperature in
the region on the 74 K transition. Right: The specific heat
versus temperature in the region of the 111 K transition. 97
4.8 (o): The electron paramagnetic resonance signal of TiPO4
versus applied magnetic field taken at 200(1) K with Hc.
Solid red line: Fit to equation 2.1. . . . . . . . . . . . . . 98
xix

4.9 Fitting parameters for the electron paramagnetic reso
nance signal of TiPO4 at 306(1) K, versus angle of the
applied magnetic field with regards to the [1,2,0]cplane.
Solid red line: Fit to a sin2() dependence. Main: The
half width at half maximum. Insert: gfactor. . . . . . . 100
4.10 (o): H [1,2,0]. (o): H c. Fitted electron paramagnetic
resonance parameters of TiPO4 versus temperature (a):
The intensity. (b): The gfactor. (c): The half width at
half maximum, the solid black (gradient 0.058(1) mT/K
and intercept 58.2(1) K) and red (gradient 0.085(1) mT/K
and intercept 59.0(1) K) lines are linear fits to the H c
and H [1,2,0] data, respectively. . . . . . . . . . . . . . 103
4.11 The spin exchange pathways and the four spin configu
rations for which the total energy has been calculated by
GGA+U calculations. Relative energies in parentheses
given in meV, first for U = 2 eV and then for U = 3 eV.
Below the figures are the equations for mapping the ener
gies onto the aforementioned spin exchange pathways. . . 106
4.12 Predicted interatomic distances. (a): TiO6 octahedron.
(b) and (c): The two different PO4 tetrahedra. (d): Ti Ti
distances in the dimerized Ti chain. . . . . . . . . . . . . 109
xx

4.13 Magic angle spinning 31P nuclear magnetic resonance spec
tra for TiPO4 shown as parts per million (ppm) versus in
tensity (temperatures indicated on each spectrum). The
orange hashed area highlights the incommensurate con
tinuum. . . . . . . . . . . . . . . . . . . . . . . . . . . . 111
4.14 The magic angle spinning 31P nuclear magnetic resonance
peak shifts given as parts per million (ppm) and/or the
boundary edges versus temperature. Inset: The 41.1 K
spectrum. . . . . . . . . . . . . . . . . . . . . . . . . . . 112
4.15 Raman spectra of a TiPO4 crystal collected in an arbi
trary and constant orientation. The data are displayed in
descending temperature as indicated. The xaxis is bro
ken between 700 and 900 cm1. . . . . . . . . . . . . . . 114
4.16 The roomtemperature and the (offset) 15 K Raman spec
tra, red and black, respectively. In the 15 K spectrum new
peaks are indicated by asterisks. . . . . . . . . . . . . . . 115
xxi

4.17 (o) and (o): Two new lowtemperature regime Raman
modes, centered at 231 cm1 and 400 cm1, respec
tively. Upper: The development of the full width at half
maximum for both modes versus temperature. Lower:
The integrated intensity of the two modes versus temper
ature. Blue solid line: Fit to both data sets, with Tc =
125(1) K and = 0.28(3). Inset: A different representa
tion of the lower figure on a loglog plot, with 1T/Tc as
the xaxis rather than temperature. The solid blue line is
the fitted line from the lower figure. . . . . . . . . . . . . 116
4.18 Results of the refinement of the single crystal diffraction
patterns of TiPO4, solid lines are a guide for the eye. (a)
The a lattice parameter versus temperature. (b) The b
lattice parameter versus temperature. (c) The c lattice
parameter versus temperature. (d) The volume of the
unit cell versus temperature. . . . . . . . . . . . . . . . . 119
4.19 The residual electron densities, obtained from single crys
tal structure refinements of TiPO4, at different tempera
tures. The temperatures are indicated on the right hand
side. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 121
xxii

4.20 (a): (o) Measured 1.5 K neutron diffraction pattern of
TiPO4 (n = 1.8860 A). Solid red line: Calculated pattern
(Rp = 12%, reduced 2 = 12.1). Solid blue line: The off
set difference between measured and calculated patterns.
The positions of the Bragg reflections used to calculate
the pattern are marked by the green vertical bars in the
lower part of the figure. Additional peaks are indicated
by asterisks. (b): The simulated neutron diffraction pat
terns with the position of the Bragg reflections marked by
vertical bars for the Cmcm and Pmmn structures, black
and red, respectively. . . . . . . . . . . . . . . . . . . . . 123
xxiii

List of Tables
1.1 The half width at half maximum for known lowdimensional
chain compounds as shown in figure 1.11, taken from the
work by Oshikawa and Affleck. . . . . . . . . . . . . . . . 24
1.2 The refined coefficients of the Pade approximation in equa
tion 1.3, as shown in figure 1.14, . . . . . . . . . . . . . . 31
3.1 Atomic positional parameters of CuCrO4 (space group
Cmcm ) as obtained from a profile refinement of the xray
powder diffraction pattern collected at room temperature.
The lattice parameters amount to a = 5.43877(50) A,
b = 8.97225(83) A and c = 5.89044(55) A. . . . . . . . . 53
xxiv

3.2 The spin exchange parameters of CuCrO4 as found by
GGA+U calculations with the two different onsite repul
sions Ueff = 4 and 6 eV. The left column for each Ueff
contains the direct theoretical results, while the values in
the right column are the scaled theoretical results such
that Jnnn equals the experimental finding of 27 K. The
rightmost column summarizes the experimentally found
spin exchange values. The final row shows the Curie
Weiss temperatures of the scaled GGA+U spin exchange
parameters, calculated using the mean field expression;
CW =13
i
ziJiS(S+1), where zi is the number of neigh
bours with which a single atom interacts via the spin ex
change Ji, and the experimentally found values from elec
tron paramagnetic resonance and magnetic susceptibility
measurements. . . . . . . . . . . . . . . . . . . . . . . . . 75
4.1 The values for the fits to the molar magnetic susceptibility
displayed in figure 4.5, the errors are given in parentheses.
(v) and (f) denote a varied or fixed quantity, respectively. 93
xxv

4.2 Values of the spin exchange parameters J1  J3 (in K) for
TiPO4 obtained by mapping the GGA+U total energies
of the four spin configurations, see figure. 4.11, onto the
Hamiltonian details are given in the text. . . . . . . . . . 107
4.3 The predicted atomic parameters for TiPO4, in the space
group Pmmn. . . . . . . . . . . . . . . . . . . . . . . . . 108
xxvi

Introduction
The study of solid materials, their properties and their phases is known
as condensed matter physics. It is a very wide, varied, research field,
ranging from the study of single atoms on a substrate to the phase
transitions of bulk samples and beyond.
A subsection of these studies focusses on magnetic phenomena. Mag
netism is a integral part of condensed matter physics and consists of
many subfields. Initially the only known (ferro) magnetic materials
were the three ferrous transition metals, iron, cobalt and nickel and a
few naturally occurring, more complex, minerals. Later new compounds
were synthesized/discovered that had new and interesting characteris
tics.
Magnetic materials are normally discussed as either itinerant or non
itinerant. Itinerant magnets are systems where the magnetic moments
are nonlocalized. This is generally realized in metals where there is a
spin polarization of the electrons at the Fermi surface. Nonitinerant
magnets, which are the subject of this PhD thesis, have a well defined
magnetic moment and are typically insulating materials. Here I concen
trate on 3d transition metal oxides where the interplay of spin, charge
and orbital degrees of freedom can result in a plethora of magnetic prop
xxvii

erties.
For 3d ions with open shells magnetism and hence the magnetic mo
ment can be rather well understood within the RusselSaunders coupling
scheme. Here S is the spin, an intrinsic property of a particle (1/2 for
an electron), and L is the angular momentum. Both are good quan
tum numbers. For f electrons, namely the 4f Lanthanoids and to some
extent also the 5f Actinoids series, the magnetic properties are best de
scribed by the quantum number J which is the total angular momentum.
The total angular momentum of the groundstate is, for the less than
half full occupation of the f levels, the absolute value of the difference
between L and S , L  S , and the sum of L and S for the more than
half full situation, i.e. L + S  . However, for the transition metals, the
3d, 4d and 5d series, the magnetic properties can often be well described
by using spin only because of the quenching of the orbital angular mo
mentum. This PhD thesis will only concern itself with the magnetism of
3d transition metals, hence only the quantum number S is of relevance.
The work that follows concentrates on nonitinerant transition metal
compounds that exhibit characteristics of onedimensional magnetism.
The first chapter will concentrate on characteristics of onedimensional
magnetism, some phenomena of onedimensional magnets and some known
compounds. The second chapter will describe the experimental and com
xxviii

putational methodology used for the investigations reported here. The
third and fourth chapters focus on the presentation of two new magneti
cally onedimensional systems, CuCrO4 and TiPO4. Despite both being
essentially isostructural and S = 1/2 systems they exhibit very different
magnetic properties.
xxix

Chapter 1
Magnetism
In this chapter I will discuss some elementary concepts of magnetism and
then focus in more detail on low dimensional magnetism. In particular
aspects of multiferroicity and other systems, that are pertinent to my
PhD work, will be reviewed.
1.1 Magnetism
Magnetism is a wide and vivid research area. This thesis will concentrate
on a small subsection of the vast field of physics, namely on 3d non
itinerant, onedimensional magnetism. Here 3d refers to the electrons
that contribute to the magnetism of transition metals. Nonitinerant
means that the magnetic moment is confined to an atom or atoms. This
1

is the case for nonconducting materials. More information can be found
in many condensed matter text books [1, 2, 3].
1.1.1 The magnetic moment
For many transition metals the magnetic moment is best described by the
spin quantum number S. Scaling linearly with the gfactor the effective
magnetic moment, which enters into the Curie law is given as
eff = g
S(S + 1).
The magnetic susceptibility (T) of a set of free uncoupled spin entities
is given by the Curielaw:
(T) =C
T
with
C =NA
2eff
3kB.
In the case of exchange interaction between the magnetic centers the
magnetic susceptibility is given by the CurieWeiss law
(T) =C
T .
Provided that the thermal energy kBT is significantly larger than the
exchange interaction energy. The CurieWeiss temperature is given by
=1
3
i
ziJiSi(Si + 1)
2

where zi is the number of neighbours with which a single atom interacts
via the spin exchange Ji.
It the temperature becomes comparable with the typical spin exchange
interaction energy one generally encounters magnetic ordering phenom
ena. These depend on many details of the lattice arrangement, crystal
anisotropies. Magnetic ordering phenomena on highly anisotropic lat
tices, i.e. lattices in which spin exchange interactions along a special
direction are predominant, are the subject of this thesis. Generally, one
encounters regimes of extended shortrange correlations before at suffi
ciently lowtemperatures longrange magnetic ordering appears.
The electronic gfactor is 2, but values slightly greater or smaller than 2
are seen for real systems since spinorbital coupling perturbs the system
in such a way that;
geff = g f( . . .)
here f( . . .) scales linearly with , the spinorbital coupling constant.
The absolute value of generally increases as one progresses through
the transition metal series, with the exception of S = 5/2 (Mn2+ or
Fe3+) where it is effectively zero. The sign of the spinorbital coupling
also changes as on progresses through the transition metal series. For
transition metals with less than half filled shells, e.g. Ti3+, is positive,
but for the more than half filled shells, when one is dealing with quasi
3

particles (holes), is negative. As such one expects a gfactor of slightly
less than 2 for Ti3+ and more than 2 for Cu2+.
1.1.2 Crystal electric field
For a free 3d transition metal atom one finds a surrounding spherical
electron cloud with all 5 3d states degenerate in energy. But when that
atom is put into a material the 3d electron clouds distort and the energy
levels are no longer degenerate. This is the effect of the crystal electric
field of the other surrounding ions. It originates from an electrostatic
interaction. When a transition metal is in an oxygen octahedral envi
ronment the 5 3d states are split into a doublet, eg, higher in energy and
a triplet t2g that is lower in energy, the former can be filled by 4 and
the latter by 6 electrons. An elongation or compression of the octahedra
results in a further splitting of the energy levels. The 3d orbitals and
the orbital energy landscape are shown in figure 1.1.
4

(a)
(b)
(c)
Figure 1.1: Taken from magnetism and magnetic materials by J. M. D. Coey [1].(a):
The five orbitals of the 3d transition metals. (b): The energy splitting of the 3d orbitals
(from left to right); a free atom, an atom in a triangular based pyramid environment, an
atom in a nondistorted octahedral environment and an atom in a cubic environment.
(c): The energy landscape of the 3d orbitals in an elongated (left) and a compressed
(right) octahedral environment.
The Pauli exclusion principle states that electrons with the same quan
tum numbers can not occupy the same space. Hence, each orbital can
5

accommodate two electrons one with spin up and one with spin down.
The electrons fill the orbitals starting with the lowest one in energy.
It is not always energetically advantageous (due to Coulomb repulsion)
for two electrons to occupy the same orbital. In some cases the elec
trons half fill the lowest energy orbitals and then continue to half fill the
higher energy orbitals. This is known as the highspin configuration and
it is common for some magnetic atoms e.g. Fe3+ and Mn2+. When the
electrons totally fill the lower energy orbitals first the arrangement is
known as the lowspin configuration. This is shown in figure 1.2. More
information can be found in most magnetism text books [4].
Figure 1.2: A pictorial representation of the high and lowspin configurations for Fe3+.
1.1.3 Interactions
Exchange interactions are integral to longrange magnetic ordering. They
can take many forms: RudermanKittelKasuyaYosida (RKKY) inter
6

action, direct exchange, double exchange and superexchange to name a
few. Here I will introduce the three forms of exchange that are pivotal
to nonitinerant magnetism and this PhD work.
Direct exchange
When neighbouring magnetic atoms interact with each other directly it
is known as direct exchange. This is not normally the case since direct
exchange requires a strong overlap of electron wave functions. Direct
exchange can be described for two Hydrogen atoms. Each atom has one
electron. When these atoms are in close proximity to one another they
find it energetically favorable to bond and this form a singlet ground
state. This is shown pictorially in figure 1.3.
Figure 1.3: A graphical representation of the radial wave functions of the free, bonded
and antibonded states of the H2 molecule. Taken from Magnetism in Condensed
Matter Physics by S. Blundell [2].
7

Mediated exchange
Mediated exchange, sometimes also known as superexchange, indirect
exchange or KramersAnderson superexchange, is exchange between two
magnetic atoms mediated through a diamagnetic only atom such as O2
or F. It acts over a longer distance than direct exchange and it is
integral to most nonitinerant magnets. It arises from the hybridization
of the transition metals d electrons and the mediators p electrons. A
p electron hops from the O2 or F to the transition metal in the same
manner as for the direct exchange mechanism. A d electron from the
other transition metal atom the hops into the empty p hole. This creates
an excited state, which relaxes when the p electrons return to the O2
or F orbitals. The sign of the exchange is governed by the orbitals
involved and their arrangement with regards to one another. This can
be seen as two direct exchange pathways. The exchange pathways can
become very large, sometimes including an additional direct O2 O2
or F F exchange.
Anisotropic exchange terms
The interaction between two spins can generally be given by
H = S i J i,j S j,
8

where J i,j is a 33 tensor that contains all information pertaining to the
spin exchange interaction. The tensor can take the decomposed form,
J i,j = T i,j + Ai,j.
Here T i,j is the symmetric component of J i,j and Ai,j is the antisym
metric component. This is an important relativistic spin exchange inter
action is known as the DzyaloshinskiMoriya (DM) interaction. It takes
the form of an extra term in the exchange Hamiltonian given by
HDM = 1
2
ij
Dij S i S j,
here the DM interaction is represented by the DM vector, Dij. A non
zero DM vector generally requires a lowsymmetry environment with
the absence of an inversion center. DM interactions are reported to play
a major role in onedimensional chain compounds and other transition
metal oxides and could possibly give rise to multiferroicity [5, 6].
1.1.4 Spin models
In a simple interpretation, spin models can be classed by the dimension
ality of the spin. The simplest onedimensional spin model is known as
the Ising model. This is where an infinite easy axis anisotropy confines
the magnetic moments to z direction. The twodimensional model,
called the XY model, occurs when an easy plane anisotropy confines the
9

magnetic moments to the xy plane. In this case there is no z axis com
ponent of the magnetic moment entering into the exchange Hamiltonian.
The final, threedimension model, the Heisenberg model, is isotropic and
has components of the magnetic moment in all three cartesian coordi
nates.
In a formal sense spin models are better described by the spin Hamilto
nian;
H =i,j
Jxxij Sxxi Sxxj + J
yyij S
yyi S
yyj + J
zzij S
zzi S zzj .
The Ising system is the special case for which one spin exchange term is
finite and the other two are zero. The XY model is obtained when two
spin exchange terms are finite, but not necessarily the same, and the
third is zero. The threedimensional case is encountered when all three
terms are finite. For the isotropic Heisenberg model they are restricted
to be the same.
1.2 Onedimensional magnetism
A system is considered to be a onedimensional magnet when it has
an infinite chain of interacting magnetic atoms running through crystal
structure. Each magnetic atom interacts with nearestneighbours along
the chain via an interchain spin exchange.
10

It is a common occurrence that within the chain the nearestneighbour
(nn) atoms generally interact strongly. However, the next nearestneighb
our (nnn) atoms can, in some cases (that will be discussed later), also
interact via a strong, if not stronger, spin exchange interaction. The nn,
nnn spin exchange interactions are indicated pictorially in figure 1.4.
nn
nnn
Figure 1.4: A simplified onedimensional chain of atoms, with the nn and nnn spin
exchange interactions indicated.
In the situation of nn, nnn antiferromagnetic spin exchange interactions
the system becomes frustrated and not all spin exchange interactions can
be satisfied simultaneously. This is demonstrated in figure 1.5. Frustra
tion can also result from nn ferromagnetic and nnn antiferromagnetic
spin exchange interactions.
11

AFM
AFM
?
Figure 1.5: A pictorial representation of a frustration in onedimensional lattice.
Onedimensional magnetism shows itself in many different ways, some
of which will be discussed below. A characteristic is a broad hump in
the magnetic susceptibility as shown for a uniform nn nonalternating
Heisenberg spin chain in figure 1.6. The hump is due to shortrange
magnetic correlation. It has been rigorously proven by MerminWagner
that for truly onedimensional systems and twodimensional Heisenberg
magnets there is no longrange ordering at finite temperature [7]. This is
why there is no sudden drop in the magnetic susceptibility in figure 1.6.
For real systems there is generally a drop or kink in the magnetic sus
ceptibility due to longrange magnetic ordering. This will be discussed
later.
12

Figure 1.6: The magnetic susceptibility of a uniform nn Heisenberg spin chain with
Jnn = 1 and a gfactor = 2, calculated using the Pade approximation put forth by
Johnston et al. [8].
1.2.1 Multiferroicity
A multiferroic is a material that exhibits more than one form of order,
e.g. anti/ferromagnetic, anti/ferroelectric and or anti/ferroelastic or
dering [9]. Multiferroics can be split into two groups, typeI and typeII.
TypeI, or proper multiferroics, are systems which have two or more in
dependent ferroic subsystems. These materials have two or more order
parameters that are not coupled with one another and appear at dif
13

ferent temperatures. Well known examples include BiMnO3 or PbVO3
[10, 11]. More pertinent to this work are typeII multiferroics, tradi
tionally referred to as improper multiferroics. Within these systems,
ferroelectricity does not exist independently of magnetic order [12, 13].
For spin 1/2 systems ferroelectricity can be the result of a helicoidal spin
density wave, for which inversion symmetry is broken upon entering the
longrange ordered states [5]. At the phase transition, longrange order
ing, the sample goes from paramagnetic and dielectric to a magnetically
ordered ferroelectric. It has been formulated by Katsura, Nagaosa and
Balatsky and Mostovoy [14, 5] that for such a case a relationship ex
ists between the electrical polarization P , the vector e12 connecting the
two spins S1 and S1 and the cross product of the magnetic moments of
neighbouring spins [S1S2], as given by;
P e12 [S1 S2].
1.2.2 Some known lowdimensional S = 1/2 quantum spin
chains
Helicoidal magnetic ordering can be realized in onedimensional systems
which have competing nn and nnn spin exchange interactions. Figure
1.7 demonstrates the phase diagram of nn, nnn spin exchange inter
actions on a onedimensional lattice. The phase diagram is split into
14

three sections. An antiferromagnetic phase exists between Jnnn = 0
with Jnn antiferromagnetic and approximate values corresponding to
the MajumdarGhosh line (MG). The MajumdarGhosh line [15, 16] is
when the nn and nnn spin exchange interactions are antiferromagnetic
and Jnn = 2Jnnn. At this special line the spin Hamiltonian;
E = Jnn
i=1
Si Si+1 +Jnn2
i=1
Si Si+2,
can be solved exactly. This point is generally accepted as the bound
ary between the antiferromagnetic and the frustrated phases. The sec
ond phase, where a helicoidal spin structure and hence multiferroicity
should exist, continues from the MajumdarGhosh line to approximately
Jnnn/Jnn = 0.25 whereupon there is a first order transition into a ferro
magnetic state, the FF point [17, 18]. The remaining segment is taken
up by the ferromagnetic phase.
To date a number of nn nnn spin chains are known. A few pertinent
systems that have attracted a lot of attention in recent years are in
cluded in figure 1.7. Except for the one inelastic neutron scattering
result for LiCuVO4, which is indicated by LiCuVO4 INS, all other spin
exchange parameters are based on density functional theory calculations
taken from various sources, as indicated in the figure caption. Hence
the results are displayed as sections rather than points, since the spin
exchange interactions have been calculated for multiple values of the
15

onsite repulsion, U .
Figure 1.7: The nn nnn spin exchange phase diagram for S = 1/2 onedimensional
system, adapted from Bursill et al. [17]. The coloured sections/lines are density func
tional theory calculations for real systems, except the line labeled LiCuVO4 INS which
is based on an inelastic neutron scattering results [19, 20, 21, 22, 23, 24].
Some examples of multiferroic systems are described in more detail be
low.
16

LiCuVO4
LiCuVO4 is a well known intrinsically lowdimensional typeII multifer
roic [19, 23, 25, 26]. At 2.4 K LiCuVO4 undergoes longrange order
ing and becomes multiferroic. It has been reported to have a helicoidal
spin spiral structure with ferromagnetic nn and antiferromagnetic nnn
spin exchange interaction [25]. The multiferroicity is evidenced by an
anomaly in the dielectric properties and a spontaneous electrical polar
ization, as shown in figure 1.8.
Figure 1.8: Main (o): The relative dielectric constant of LiCuVO4 versus temperature.
Inset (o): The electrical polarization of LiCuVO4, calculated from the pyroelectric
current, versus temperature. Taken from Schrettle et al. [26].
17

CuCl2
CuCl2 was the subject of many investigations which probed its multifer
roic behaviour at lowtemperature [20, 27]. CuCl2 undergoes longrange
ordering at 23.9(1) K as evidenced by specific heat, magnetic suscep
tibility and elastic neutron scattering experiments, see figure 1.9 and
the citation(s) therein. At longrange ordering a sharp spike is seen
in the dielectric constant below which there is a spontaneous electrical
polarization. At lower temperatures, immediately below the longrange
ordering anomaly, the relative dielectric constant starts to grow. With
decreasing temperature it levels off and then starts to decrease. This
has the appearance of a broad asymmetric hump. With the application
of a magnetic field the spike does not change but the hump decreases
in size and moves to higher temperatures. The dielectric constant and
spontaneous polarization are displayed in figure 1.10.
18

Figure 1.9: Main (o): The molar magnetic susceptibility of CuCl2 measured in a
magnetic field of 1 T versus temperature. Inset (o): A loglog plot of the specific heat
of CuCl2 versus temperature. All results taken from Banks et al. [20].
19

Figure 1.10: Main (o): The relative dielectric constant of CuCl2 versus temperature,
for various magnetic fields. Inset (o): The electrical polarization of CuCl2, calculated
from the pyroelectric current, versus temperature. Taken from Seki et al. [27].
TiOX (X=Cl or Br)
The compounds with composition TiOX (X=Cl or Br) have drawn much
attention recently, since both compounds have a twostep spinPeierls
transition [28, 29, 30, 31, 32, 33]. The magnetic susceptibilities of both
materials are dominated by a broad hump at high temperatures indica
tive of onedimensional short range antiferromagnetic correlations. At
lower temperatures there are two subsequent sharp decreases of the mag
20

netic susceptibility, leaving only a finite van Vleck plus diamagnetic con
tribution and a small paramagnetic impurity. The spinPeierls transition
in both compounds happens in two steps: The first transition (drop in
magnetic susceptibility at 92 and 47 K for the Cl and Br compounds,
respectively) is a second order or continuous transition from a param
agnetic phase into a structurally incommensurate phase. At the second
transition at 67 and 28 K for Cl and Br, respectively, a drop in magnetic
susceptibility is observed. At lowest temperature both samples become
fully dimerised. This transition is first order and hysteretic in nature. A
new crystal structure has been reported for TiOCl below 28 K [34]. For
more information see the cited articles.
1.2.3 Interchain couplings and longrange ordering
Generally, weak interchain spin exchange interactions, J, lead to long
range magnetic ordering at sufficiently lowtemperatures. One can es
timate the interchain coupling from the longrange ordering tempera
ture. Yasuda et al. calculated the Neel temperature (TN) of a quasi
onedimension Heisenberg antiferromagnet on a cubic lattice with the
isotropic interchain coupling J, inducing threedimensional longrange
magnetic ordering at TN [35]. By scaling their quantum Monte Carlo
simulations they extrapolate for infinite system size, a relationship be
21

tween inter and intrachain coupling, given by;
TN/J = 0.932ln(A) +
1
2ln(ln(A)), (1.1)
where A= 2.6 J/TN and J is the intrachain spin exchange constant.
1.2.4 Electron paramagnetic resonance theory
Oshikawa and Affleck [36, 37] developed a theory for the electron para
magnetic resonance of S = 1/2 quasionedimensional chain compounds
at lowtemperatures which have anisotropic or antisymmetric exchange
terms i.e. Jxx = Jyy = Jzz. At lowtemperatures near longrange
ordering they found that there is a positive linear slope of the line
width with increasing temperature. The proportionality constant de
pends upon many aspects and as such no quantitative results can be
obtained easily. But there is a system independent factor of 2 between
the proportionality prefactors parallel and perpendicular to the easy
axis. Such as;
weasy axisweasy axis
= 2,
where,
w =(HWHM)
T.
22

They went on to demonstrate this for some known chain compounds.
Their published comparisons are displayed here in figure 1.11. The re
ported temperature dependencies are tabulated in table 1.1.
Figure 1.11: The electron paramagnetic resonance normalised linewidth versus reduced
temperature for CuGeO3, KCuF3 and NaV2O5 shown against a linear line. The graph
is taken from the work by Oshikawa and Affleck [37].
Prior to the work by Oshikawa and Affleck, Kubo and Tomita reported
that for S = 1/2 antiferromagnetic nn chain systems the saturation of
linewidth at hightemperatures could be due to the anisotropic or anti
symmetric spin exchange interactions [38]. Defining as the deviation
from the isotropic exchange such as,
Jzz = Jxx (1 ),
they put forth the relationship in equation 1.2, where Jnn is the nn spin
23

w (T/K) Compound Orientation
4.2104 CuGeO3 Bc
4.7104 CuGeO3 Ba
17104 KCuF3 Bc
22104 KCuF3 Ba
1.3104 NaV2O5 Bc
0.65104 NaV2O5 Bb
Table 1.1: The half width at half maximum for known lowdimensional chain com
pounds as shown in figure 1.11, taken from the work by Oshikawa and Affleck [37].
exchange, and H is half linewidth at half maximum of the electron
paramagnetic resonance absorption line.
H(T ) 2
gBJnn(1.2)
Now that I have given an introduction to onedimensional magnetism I
will discuss as a first result a Pade approximation for the temperature
dependence magnetic susceptibility of a S = 32 Heisenberg quantum anti
ferromagnetic spin chain.
24

1.2.5 Pade approximation for the molar magnetic susceptibil
ity of a S = 32 Heisenberg quantum antiferromagnetic
spin chain
Onedimensional magnetic systems can be characterized by magnetic
susceptibility, see section 1.2. Being able to model the temperature
dependent magnetic susceptibility of a onedimensional system is very
helpful since values such as the nn spin exchange interaction and the
gfactor can be ascertained.
A Pade approximation is a useful tool in mathematics to approximate a
given function. Pade approximations have been widely used in modern
condensed matter physics for fitting observables, e.g. the molar magnetic
susceptibility or specific heat. A well known and highly cited example
is the Pade approximation for the molar magnetic susceptibility and the
specific heat of a S = 1/2 Heisenberg alternating chain, as put forth by
D. C. Johnston et al. [8]. Within the paper Johnston et al. discussed a
nonalternating S = 1/2 Heisenberg chain. In the spirit of Johnstons
work, the Pade approximation for the magnetic susceptibility of a S = 32
Heisenberg quantum antiferromagnetic spin chain was formulated from
results obtained by quantum Monte Carlo simulations for a S = 3/2
Heisenberg chain.
25

A Pade approximation is given by;
f(x) =
1 +mi=1
Ai xi
1 +n
j=1
Bj xj.
Here both summations include sufficient terms to approximate the func
tion to the desired accuracy such that the difference between the Pade
approximation and the calculation is similar if not smaller than the error
resulting from the quantum Monte Carlo simulations.
For the Pade approximation already discussed and the new approxima
tion put forth here, f(x) is the spin susceptibility multiplied by S(S+1)
and x is Jnn/T or the reciprocal reduced temperature. Hence the ap
proximation now takes the form of;
(Jnn/T ) =
1 +mi=1
Ai (Jnn/T )i
1 +n
j=1
Bj (Jnn/T )j. (1.3)
Here
mol(Jnn, g, T ) = (Jnn/T )
NA2Bg
2
kB Jnn.
Previous to this work, Pade approximations for all possible spins of the
transition metal series, i.e. S = 1/2 5/2, were put forth in the PhD
thesis of S. N. Grossjohann [39]. However, the system size chosen was
26

rather small, 512 spins and as such the results severely suffered from
finite size effects at relatively high temperatures. Previous to the work
by Grossjohann a trivial approximation was put forth by Hiller et al. [40].
Previous to all of these works, Fischer put forth a classical approximation
for any spin system [41]. A comparison of the three previous works
pertaining to the temperature dependent magnetic susceptibility of a
S = 3/2 spin chain and our quantum Monte Carlo calculations are shown
in figure 1.12. The previous nonclassical work suffers from finite size
effects and the quantum Monte Carlo results being reported here are
more accurate and closer to the true temperature dependent magnetic
susceptibility of such a chain. A S = 3/2 system is best described as
being a quantum spin system and as such the classical approach does
not describe the system adequately.
27

0 10 200.5
1.0
1.5
2.0 QMC 2000 spins Grossjohann SSE 512 spins Classical approximation Hiller et al. approximation
S
(S+1
)(101
)
kBT/JNNFigure 1.12: (o): Our quantum Monte Carlo results, see text for more information.
Solid blue line: The Pade approximation by Grossjohann [39]. Solid green line: The
classical approximation put forth by Fischer [41]. Solid black line: The approximation
by Hiller et al [40].
The modified spin susceptibility for a S = 3/2 antiferromagnetic Heisen
berg spin chain was calculated using the looper algorithm on a cluster
within the ALPS suite. For more details see section 2.6.1. Initially the
magnetic susceptibility was calculated at sufficiently low values of T/Jnn
for different system sizes, so as to ascertain a system size that would
be acceptable to reproduce what would be observed for a real system
(N NA), the results are shown in figure 1.14 insets b. A system size
28

Figure 1.13: Left: The scaled computation time versus system size at a reduced tem
perature of 0.05. Right: The arbitrary computation time versus spin, at a reduced
temperature of 0.05.
of N = 2000 was chosen, since for systems sizes N 2000 converging
values of the spin susceptibility were obtained within error bars, see fig
ure 1.14 (b). Bigger systems could have been chosen but this would
have drastically increased computation times for little gain. The scaling
of computation time with both system size and spin can be seen in fig
ure 1.13. A clear nonlinear scaling can be seen for both variables, the
system size scaling is exponential as one would expect.
29

0 10 200.5
1.0
1.5
2.0
101
kBT/JNN
0 10 202
1
0
1
2
(b)
calc
pad
10
4
kBT/J
NN
(a)
0 1000 2000 30006.0
6.2
6.4
6.6
calc
102
N
kBT/JNN=0.05
Figure 1.14: Main: (o): The temperature dependent modified spin susceptibility for a
S = 3/2 spin chain with nn spin exchange interactions, calculated by quantum Monte
Carlo using the ALPS suite, versus reduced temperature. Solid red line: A fit to a Pade
approximation as discussed in the text. (a): (o): The difference between the modified
spin susceptibility as calculated by quantum Monte Carlo and the Pade approximation
fitted to the simulation. The solid red lines denotes the boundaries of the error bars
given for the quantum Monte Carlo calculation. (b) The modified spin susceptibility for
different systems sizes at a fixed reduced temperature of 0.05. N denotes the number
of spins.
30

i/j Ai Bj
1 68.72481 489583.7
2 613928.0 1.89146E6
3 805554.35929 3.86820E6
4 703853.6 6.07049E6
5 394585.7 2.81538E6
6 21142.94 645334.4
7 872.0836 23234.23
8 78.03424 431.4632
9 4.440790 1.928260
10 0.067570 0.1536200
11 0.008050 2.24279E5
12 2.742790E4 1.75778E4
Table 1.2: The refined coefficients of the Pade approximation in equation 1.3, as shown
in figure 1.14, .
The modified spin susceptibility was fitted to the aforementioned ap
proximation with reduced 2 values of 1.21 and an adjusted R2 of 1.00.
The fit can be seen in figure 1.14 with the difference between calculated
and fitted values shown in inset (a). The temperature dependent error
of the quantum Monte Carlo results are indicated by the two red lines.
The terms of the Pade approximation up to the 12th order are tabulated
in table 1.2.
31

1.3 Summary
In this chapter I discussed multiferroicity and lowdimensional mag
netism with an emphasis on what is relevant for this PhD thesis. I
also discussed relevant materials that will be commentated on in the
following chapters.
The next chapter will give a brief overview of experimental methodology
and computation that will be used to characterize CuCrO4 and TiPO4
in the latter chapters.
32

Chapter 2
Experimental methodology and
computation
In this chapter I will discuss and explain the experimental methodology
and computations that were used to characterize the systems reported
on in the following chapters. This chapter is meant to be a concise
experimental overview. More information can be found in the pertinent
manuals and the published papers.
33

2.1 Xray and neutron diffraction
2.1.1 Single crystal diffraction
CAD4 diffractometer
CAD4 is a four circle diffractometer manufactured by Enraf Nonius, that
allows data acquisition from 0 2 and 0 . It employs non
monochromated Ag radiation (0.5608 A). The machine was primarily
used for orientating single crystals.
STOE IPDS diffractometer
The STOE IPDS diffractometer is a two circle diffractometer. It uses an
imaging plate detector which allows data acquisition from 0 2.
It uses nonmonochromated Ag radiation (0.5608 A). The machine was
primarily employed for crystal structure determination.
2.1.2 Powder diffraction
Labbased xray diffractometers
Two xray powder diffractometers were used, both STOE Stadi P ma
chines. One machine produced monochromated Cu xray radiation (Cu
34

K1 1.54056 A) and the other used monochromated Mo xray radi
ation (MoK1 0.70930 A). Both are equipped with Germanium(111)
monochromators, and as such both select fully monochromated K1 ra
diation. The advantage of having access to MoK1 is such that it allows
one to measure elements that would absorb the frequently used Cu radia
tion, e.g. Cr. The samples were mounted in thin walled quartz capillaries
( = 0.3 or 0.1mm). This technique allows for preparation in a glove
box and hence patterns of air sensitive samples could be easily collected
[42].
High resolution powder diffractometer for thermal neutrons  HRPT
HRPT is a high resolution thermal neutron powder diffractometer. It
was designed for small samples and has a resolution comparable to those
of synchrotron xray powder diffraction studies, with a possible resolu
tion of 0.05. The machine is located at SINQ in the Paul Scherrer
Institute, Switzerland. A schematic can be seen in figure 2.1.
35

Figure 2.1: Schematic of the powder diffractometer HRPT at the Paul Scherrer Insti
tute (Switzerland) [43].
2.2 Magnetisation
2.2.1 SQUID magnetometry
Magnetisation was measured using a Quantum Design Magnetic Prop
erty Measurement System, or MPMS for short. The machine allows the
measurement of magnetisation in the range of 7 T in the temperature
range 1.85 K to 400 K. An additional oven insert enables measurements
36

in the higher temperature range of 300 K to 800 K. The sample, whether
it is a powder or crystal, was generally mounted in the sample holder by
two different methods. The simplest and fasted method has the sample
contained within a diamagnetic only gelatine capsule, which weighs ap
proximately 40 mg. The raw magnetisation could then be later corrected
for the magnetisation of the sample holder. A gelatine capsule is shown
in figure 2.2. The second, more time consuming method, was mounting
the sample in a suprasil c quartz tube. The tube is thin walled, so as
to add the smallest background signal possible. It is sealed half way
up its length, in a manner that deforms the longitudinal distribution
of weight as little as possible, i.e. the longitudinal mass distribution
(mg/cm) remains relatively constant. This could never be fully guaran
teed, but measurements of the magnetisation of such a sealing yielded a
magnetic susceptibility of 109 emu/Oe for which the raw data could
be corrected. Once the sample was mounted, the tube was evacuated
and flushed with helium gas a few times. This ensured that there was
no O2 gas that would give an additional signal at lowtemperature and
provide a good thermal contact to the cryostat. The tube was finally
sealed. A sealed tube and the seal half way up the tube are displayed in
figure 2.3.
37

Figure 2.2: Left: A filled gelatine capsule as used for measuring the magnetization.
Right: A disassembled, empty, gelatine capsule, prior to use for measuring magnetiza
tion.
Figure 2.3: Left: A filled and sealed quartz tube ready for magnetization measurements.
Right: A closer view of the seal half way up the tube.
38

The molar magnetic susceptibility could be calculated from the raw mag
netisation by
mol[cm3/mol] =
M(T,H)[emu]m[g]Mm[g/mol] H[Oe]
where M(T,H)[emu] is the measured magnetisation, m[g] is the mass of
the sample, Mm[g/mol] is the molar mass of the sample and H[Oe] is the
applied magnetic field.
The magnetic susceptibility also required correcting for the diamagnetic
contribution resulting from the closed shells of the atoms contained
within the sample. The values are well known and tabulated by Sel
wood [44]. An example which is relevant to this work would be Cu2+
which has a diamagnetic contribution of 11 106 cm3/mol.
In addition to the diamagnetic signal of the samples, an additional pos
itive temperature independent van Vleck contribution also needed to be
subtracted from the magnetic susceptibility. The van Vleck contribu
tion, sometimes referred to as the van Vleck temperature independent
paramagnetism, arises from the population of the magnetic states that
are higher in energy than the magnetic ground state. As such, it is sys
tem specific quantity. For Cu2+ it typically amounts to values between
20 106 cm3/mol and 120 106 cm3/mol depending on the direction
39

of the applied magnetic field with respect to the crystal axes.
2.3 Specific heat
2.3.1 Relaxation calorimetry
Specific heat was measured using a Quantum Design Physical Property
Measurement System (PPMS), via the relaxation technique. The ma
chine allows the measurement of multiple physical properties, but for this
work only the specific heat option was used. The specific heat was mea
sured in the magnetic field range of 9 T and in the temperature range
of 1.85 K to 350 K. An additional 3He insert allows one to measure down
to 400 mK. Crystals were mounted to a thermally decoupled sample
holder by Apiezon c vacuum grease. A premeasurement, an addenda
measurement, was done before mounting the sample so that the specific
heats of the sample holder and the Apiezon c vacuum grease could be
subtracted from the total specific heat, yielding the specific heat of the
sample.
Powders could also be measured on a PPMS sample holder, either by
pelletizing and mounting it in the same way as crystals or by slightly
melting the Apiezon c grease, once the addenda has been measured, and
adding the powder. The slightly molten Apiezon c vacuum grease would
40

allow the powder to sink into it and thermally anchor the sample. A
typical sample investigated by this method weighed approximately 2 mg.
2.3.2 Adiabatic Nernst calorimeter
A home built quasiadiabatic Nernsttype calorimeter was also used. It
allowed one to measure specific heat in the temperature range 2.0 K to
300 K. The machines construction and testing has been the subject of M.
Banks PhD thesis [45]. The calorimeter can accommodate single crystal
and powder samples. The powder samples were first housed in a flat
bottom high purity glass bell jar filled with helium gas. The mass of the
glass must be known so it can be subtracted later from the total specific
heat. An empty and full glass bell jars are shown in figure 2.4. This is
discussed in depth in M. Banks thesis. The sample, be it a powder or
a single crystal, is then attached to a thermally isolated sapphire plate,
which has a heater and a calibrated thermometer, via Apiezon c vacuum
grease. See the aforementioned thesis for more details.
41

Figure 2.4: Top: An empty glass bell jar. Bottom: A full sealed glass bell jar, ready
for specific heat measurements; left is a view from the top and right is a view from the
side.
2.4 Electron Paramagnetic Resonance spectroscopy
The electron paramagnetic resonance spectra were collected on a home
built microwave spectrometer. The spectrometer operates at 9.5 GHz
(Xband). The required field was created by an iron core Bruker BE25
magnet equipped with a BH15 field controller. The cryostat is a contin
uous flow system and can operate in the range of 3 K to 295 K. There
are two sample mounts. The first is an electron paramagnetic resonance
neutral lowbackground suprasil c quartz tube. The second is an elec
42

tron paramagnetic resonance neutral mount with an attached calibrated
temperature sensor (Cernox CX 1050) next to the sample. The sensor
is shielded by a gold foil so as not to create an additional electron para
magnetic resonance signal. This sample holder allows for a very precise
temperature measurement next to the sample. Both samples holders are
shown in figure 2.5.
Figure 2.5: Left: The electron paramagnetic resonance sample holder with a mounted
temperature sensor. Right: The electron paramagnetic resonance neutral low
background suprasil c quartz tube with a sample mounted.
Typically an electron paramagnetic resonance signal is the differential
of a single, or a convolution of many, lorentzian resonance peaks. The
spectrum could be fitted to the equation;
43

EPRsignal =Ni=1
d(Li(H))
dH+ y0 + y1 H+ y2 H2, (2.1)
where y0, y1 and y2 are variable background terms, N represents the
total number of peaks and L(H) is given as;
L(H) =I
w+ (H Hres)
(H Hres)2 + (w)2. (2.2)
Where I is the intensity, w is the half width at half maximum, Hres
is the resonance position and is the dispersion. When an electron
paramagnetic resonance signal is very broad, the negative field resonance
should also be included.
The gfactor can be ascertained from the resonance field Hres by
gBHres = h. (2.3)
Hence,
g =0.71449 [MHz]
Hres[G],
where is the applied microwave frequency.
44

2.5 Dielectric capacitance
Dielectric capacitances were measured with either an AndeenHagerling
AH2500A or an AH2700 capacitance bridge. Both are high precision
variable ACvoltage bridges. The latter has a variable frequency option,
50 to 20000 Hz in discrete steps, whereas the former operates at a fixed
1000 Hz frequency. Samples were mounted via two methods. The first
method, used for single crystals or pelletized powders, involved creating
contacts on either side, with silver paint/paste or by depositing gold
on the surface. Gold wires where then connected to the contacts which
in turn where soldered to coaxial copper wire that led to the bridge.
The second method applicable for powder samples only, had the powder
compacted and sandwiched between two copper pistons in a vespelr
tube. The copper pins were then in turn connected to coaxial copper
wire which led to the bridge. All measurements where done in an Oxford
helium cryostat equipped with a variable temperature insert allowing
temperatures between 1.2 K and 300 K using a 12 T superconducting
magnet.
45

2.6 Computation
2.6.1 Algorithms and Libraries for Physics Simulations  ALPS
The ALPS project (Algorithms and Libraries for Physics Simulations)
is an open source effort aiming at providing highend simulation codes
for strongly correlated quantum mechanical systems as well as C++
libraries for simplifying the development of such code. ALPS strives to
increase software reuse in the physics community. [46]
The ALPS v1.3.5 project incorporates many programs. The two most
pertinent programmes to this work are the looper code for quantum
Monte Carlo simulations [47] and the Full Diagonalization Package for
exact solutions of finite systems. The looper code allows the calcula
tion of observables such as spin magnetisation, spin susceptibility, spe
cific heat and staggered magnetisation for large (N 1000) finite sys
tems. For such large systems the observables can be assumed to be
those of an infinite system, with only very lowtemperature observables
(T/J < 0.01) showing a deviation from an infinite system, i.e. an N de
pendence for large N (N 1000). This makes quantum Monte Carlo a
very powerful tool for simulating different systems. However, the quan
tum Monte Carlo approach has a problem. When it comes to frustrated
systems it encounters the sign problem [48] and the solution does not
46

converge. This is where the second package, Full Diagonalization, comes
into play. Full Diagonalization allows one to exactly solve the hamil
tonian for a finite system and as such calculate observables. But the
system size is heavily limited by computing power and more importantly
by RAM memory capacity. As such modern computers can only solve
S = 1/2 systems for approximately 24 atoms. With larger spins the
system size has to be significantly reduced. This results in deviations
(finite size effects) at relatively large temperatures, T/J < 0.3. How
ever, with these limitations in mind Full Diagonalization can be used to
obtain observed behaviour in many systems.
2.7 Summary
In this chapter I briefly described the experimental method used for
characterization of the systems discussed in the other chapters.
In the next chapter I will be discussing our investigation of CuCrO4.
This is a chemically wellknown compound but its magnetic properties
have never been studied until now. We reported in our publication, that
CuCrO4 is a previously unknown typeII multiferroic [24].
47

Chapter 3
CuCrO4  A new multiferroic
material
In this chapter I will discuss the magnetic properties of CuCrO4, a
S = 1/2 3d9 spin chain. Here I am reporting a detailed experimen
tal and theoretical investigation characterizing the magnetic properties
of CuCrO4 for the first time.
48

3.1 Crystal structure
Figure 3.1: The crystal structure of CuCrO4, projected slightly off of the caxis. The
unit cell is doubled along the caxis. Blue octahedra: CuO6 units. Green tetrahedra:
CrO4 units.
CuCrO4 crystallizes with the CrVO4 structuretype (space group Cmcm),
with Cu and Cr in the oxidation state 2+ and 6+, respectively [49, 50].
Cu2+ has the electronic configuration 3d9 with one hole in the 3d shell,
hence S=1/2, while Cr6+ has an empty dshell. Consistent with the
other compounds which belong to the CrVO4 structuretype, the per
tinent structural feature is the corrugated CuO2 ribbon chains running
along the caxis. The ribbon chains are made up from planar CuO4
49

plaquettes which are connected via transedges, as shown in figure 3.1.
The CuO4 plaquettes form the basis of elongated (JahnTeller distorted)
CuO6 octahedra. The ribbon chains are interconnected by slightly dis
torted CrO4 tetrahedra, which inhabit interstitial voids. At room tem
perature the Cu2+ Cu2+ distance is reported to be 2.945(2) A with a
Cu2+ O2 Cu2+ angle of 97.067(7)o [50].
3.2 Sample preparation
The preparation of CuCrO4 is rather intriguing, mainly due to the insta
bility of the copperchromate 1:1:4 stoichiometry. According to Hanic
et al. at rather lowtemperatures CuCrO4 decomposes into the spinel
type CuCr2O4 and CuO [51]:
4CuCrO4687 K 773 K 2CuO + 2CuCr2O4 + 3O2.
Sofar this seriously hampered the growth of crystals, suitable for bulk
characterization, as well as the preparation of highly homogenous sam
ples.
The second problem associated with sample preparation is a health and
safety concern, Cr6+ is considered a genotoxic carcinogen [52]. As such
all samples must be handled with care.
50

Multiple methods can be employed to prepare polycrystalline sample of
CuCrO4. All measurements reported here were undertaken on a single
powder sample ( 160 mg total available sample) that was prepared
by separately dissolving equimolar amounts Copper(II) hydroxide and
Chromium(VI) oxide in distilled water. The two solutions were mixed
and boiled to dryness. The resulting powder was heat treated in air at
a temperature of 150C for 2 days. This method was first described by
Arsene et al. [53]. The phase purity of the sample was checked by xray
powder diffraction measurements using a STOE STADIP diffractome
ter with monochromated MoK1 radiation. The powder pattern was
fitted using the Rietveld profile refinement method employed within the
Fullprof Suite [54]. No other reflections besides those of CuCrO4 were
observed. The pattern and the resultant fit can be seen in figure 3.2. The
structural parameters of this fit are tabulated in table 3.1. Later, larger
samples intended for powder neutron diffraction were prepared along a
similar route replacing Copper(II) hydroxide by anhydrous Copper(II)
acetate. It should be noted that the sample is reported and was found
to be brick red in colour. But black samples, initially believed to be
decomposed samples, can also be obtained. According to xray powder
diffraction are isostructural to their red counterparts. The only differ
ence in their preparation was a longer or higher annealing temperature.
The sample was prepared by Prof. R. Glaum and his group at Bonn University, Bonn.
51

5 10 15 20 25 30 35
0.0
0.5
1.0
Co
un
ts(a
rb.u
nits)
2q ()
Figure 3.2: (o): Measured xray powder diffraction pattern of CuCrO4 ( = 0.70930 A
). Solid red line: Calculated pattern (Rp = 13.1%, reduced 2 = 1.15) using the
parameters given in table 3.1. Solid blue line: The offset difference between measured
and calculated patterns. The positions of the Bragg reflections used to calculate the
pattern are marked by the green vertical bars in the lower part of the figure.
3.3 Magnetic susceptibility
The molar magnetic susceptibility of a powder sample of CuCrO4, con
tained within a gelatin capsule was measured in the temperature range
of 2 K to 350 K in an applied dc magnetic field of 1, 3, 5 and 7 T. Above
20 K no field dependence was observed, suggesting minimal ferromag
netic impurities. However, upon cooling a noticeable field dependence
became apparent. At lowest temperatures an almost asymptotic be
52

oxidation Wyckoff position
atom state and letter x y z Biso
Cu +2 4a 0.0000(0) 0.0000(0) 0.0000(0) 0.089(8)
Cr +6 4c 0.0000(0) 0.3700(3) 0.2500(0) 0.904(7)
O1 2 8f 0.0000(0) 0.2652(5) 0.0312(9) 0.800(12)
O2 2 8g 0.2326(7) 0.0198(6) 0.2500(0) 0.800(12)
Table 3.1: Atomic positional parameters of CuCrO4 (space group Cmcm ) as obtained
from a profile refinement of the xray powder diffraction pattern collected at room
temperature. The lattice parameters amount to a = 5.43877(50) A, b = 8.97225(83) A
and c = 5.89044(55) A.
haviour was observed for small fields, with a kink at 8 K and an
illdefined shoulder ranging from 11 to 20 K. In small magnetic fields
a thermal hysteretic behaviour was seen below the illdefined shoulder.
Upon application of a larger magnetic field the molar magnetic suscepti
bility decreased and the asymptotic and hysteretic behaviour died away.
The kink became more pronounced and it is interpreted as evidence
of longrange magnetic order. The illdefined shoulder gradually faded
away and was replaced by a welldefined hump, which is indicative of
onedimensional short range correlations, with a maximum centered at
15 K.
53

Figure 3.3: The molar magnetic susceptibility of CuCrO4, in the lowtemperature
regime, versus temperature for various magnetic fields. Red symbols: Heating data.
Blue symbols: Cooling data.
At high temperature, 100 K, the molar magnetic susceptibility fol
lowed the modified CurieWeiss law;
mol(T ) =C
T + dia + vV, (3.1)
54

where C is the Curie constant pertaining to the spin susceptibility of the
Cu2+ entities. The Curie constant is given as C = NAg2 2B S(S + 1)/3kB.
dia refers to the diamagnetic susceptibilities of the electrons in the closed
shells which could be estimated from the tabulated increments given by
Selwood as 62106 cm3/mol [44]. The vV contribution can not be
tabulated and can not be calculated precisely, but values are known for
similar compounds and comparisons can be made (see above).
55

0 100 200 3000
250
500
750
1000
1/c
m(m
ol/cm
3)
T (K)
Figure 3.4: (o): The inverse molar magnetic susceptibility versus temperature of
CuCrO4, measured in a field of 7 T. Red solid line: Fit to the modified CurieWeiss
law as given in equation 3.1.
Best agreement was found with a gfactor of 2.17(2), a of 56(1) K and
dia + vV +20 106 cm3/mol. This implies a vV of +80 106
cm3/mol which is a reasonable value for Cu2+ in this environment [20].
56

Figure 3.5: (o): The 7 T molar magnetic susceptibility versus temperature for CuCrO4.
Dashed/solid lines: The simulated molar magnetic susceptibility for various cases, see
text for more details.
Below 100 K the magnetic susceptibility deviated from a CurieWeiss
law due to shortrange correlations. The temperature dependence of the
lowertemperature range can be approximated theoretically by full di
agonalization calculations of a finite system (N=20). Such results for
chain(,T) were available from HeidrichMeissner et al. [55] for from
57

+4 to 4, where =Jnn/Jnnn. Guided by density functional theory cal
culations (see sections 3.7) values of ranging from 1.5 to 2.5 were
compared to the experimental data along with the molar magnetic sus
ceptibility of a uniform nn antiferromagnetic chain [8]. Interchain spin
exchange interactions could be approximated with a meanfield correc
tion, such as
mol(T ) =chain(T )
1 chain(T )+ 0,
where is given by
=1
NAg22B
i
ziJiSi(Si + 1).
Here Ji is an interchain spin exchange interaction constant that occurrs
zi times for a given atom with spin Si. 0 can be taken from above,
+20 106 cm3/mol. A gfactor of 2.125 was used, which is con
sistent with electron paramagnetic resonance measurements, see section
3.5. Jnnn was scaled so as to reproduce the hump at the correct temper
ature. The results are shown in figure 3.5. It is apparent from the graph
that best agreement is obtained for an 2, Jnnn = 27 K and a of
7(1) mol/cm3. z1 = 4, z2 = 2 was assumed for the density functional the
ory calculations. As shown by the density functional theory calculations
58

with a of 7(1) mol/cm3 and J1 1/4J2 one finds J2 = 12(2) K. This
is in very good agreement with the experimental results (see section 3.7
and table 3.2).
A future high magnetic field experiment has been scheduled. A pulsed
magnetic field of 70 T will be applied and the magnetisation versus
field will be measured. In order to predict the results full diagonalization
of a finite (N=18) system was performed using the ALPS package (see
section 2.6.1 for details relating to the ALPS package). The system of
18 spins on a onedimensional lattice with periodic boundary conditions
was solved with nn and nnn spin exchange interactions set to the values
ascertained from magnetic susceptibility measurements( 27 K and 54 K,
respectively). The results, with a gfactor of 2.125 at 1.4 K, can be seen
in figure 3.6.
59

Figure 3.6: Full diagonalization results. Solid red and black lines are the magnetisation
and d(M)d(H)
versus applied magnetic field, respectively.
3.4 Specific heat
The specific heat versus temperature of CuCrO4 was measured on a
powder sample of 2.43 mg (see figure 3.7 and for experimental details
see section 2.3). A broad, smeared, type anomaly centered at 8.2(2) K
can be clearly seen. This is indicative of longrange magnetic ordering.
60

Within figure 3.7 there is also presented the specific heat measured with
an applied magnetic field of 9 T. The data is offset so as to be clearly
distinguishable from the 0 T data. Within error bars the data for the two
different fields are identical. This implies that the longrange ordering
anomaly does not shift as a function of applied magnetic field. The intra
chain is 27 K, this is substantially larger in energy than 9 T and as
such one would not expect a significant change of the spin arrangement.
Specific heat divided by temperature is plotted versus temperature and
it is shown in figure 3.8. This plot allows an estimation to be made
of the entropy contained within the longrange ordering anomaly. S
0.6 J/mol.K was found to be contained within the anomaly. This is
10 % of the expected total magnetic entropy for a S = 1/2 system,
S = R ln(2S+1). For S = 1/2 we obtain R ln(2), where R is the molar
gas constant. The other 90% of the entropy has been removed by short
range correlations at higher temperatures. At longrange ordering the
single ribbon chains are high correlated and most of the entropy left
pertains to the ordering of the chains with respect to each other.
61

0 4 8 120
1
2
3
4
0T
9T
Cp
(J/m
olK
)
T (K)
Figure 3.7: The specific heat versus temperature for CuCrO4. (o): 0 T data. (): 9 T
data, offset b